1. International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 –6340(Print), ISSN 0976 – 6359(Online) Volume 4, Issue 2, March - April (2013) © IAEME521DRY SLIDING STUDIES OF POROSITY ON SINTERED CU-BASEDBRAKE MATERIALSGlenn Kwabena GYIMAH1,a*, Dong CHEN1,b, Ping HUANG1,c,School of Mechanical and Automotive Engineering, South China University of Technology,Guangzhou, 510640, P. R. China.1ABSTRACTCu-based composites with its promising engineering application due to their excellentthermophysical properties coupled with better high temperature mechanical properties ascompared to pure copper and copper alloys. An investigation on a Cu-based compositefrictional material re-inforced with other elements for train brake was treated under P/M routefor its wear behavior in terms of sintering temperature and porosity. The dry sliding wearcharacteristics investigation test with a high pressure pad-on-disc tester was developed for thethree different sintering temperatures samples. The optimal porosity was obtained at thehighest sintering temperature of 950oC. That same optimal porosity gave the lowest wearfrictional coefficient, and the highest coefficient of friction. Three forms of wear mechanismswere observed during the dry sliding process, namely, delamination wear, plowing wear andabrasive wear. High wear rates were found on samples sintered at 850oC and 900oC. Abrasivewear and the delamination wear were the main cause of high wear coefficient, low wearnumber and low coefficient of friction. The nature of abrasive surfaces observed wereclassified into three divisions, namely, smooth abrasive surfaces; rough abrasive surface; andthe highly abrasive surface. The dominance of wear is discussed in the light of SEMphotography of the worn surfaces.Keywords: Brake materials; Wear; Porosity; Wear mechanism; Sintering temperature.INTERNATIONAL JOURNAL OF MECHANICAL ENGINEERINGAND TECHNOLOGY (IJMET)ISSN 0976 – 6340 (Print)ISSN 0976 – 6359 (Online)Volume 4, Issue 2, March - April (2013), pp. 521-529© IAEME: www.iaeme.com/ijmet.aspJournal Impact Factor (2013): 5.7731 (Calculated by GISI)www.jifactor.comIJMET© I A E M E
2. International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 –6340(Print), ISSN 0976 – 6359(Online) Volume 4, Issue 2, March - April (2013) © IAEME5221. INTRODUCTIONRecently, much attention has been given to the effect of porosity on Cu-based matrixcomposites, due to its indispensable influence on tribological and mechanical behavior ofsintered composites. The influence of Porosity is very high in the determination of amaterial’s application. The porosity of material influences its ability to withstand wear sinceit has an impact on the properties of the Cu-based composite material. In view of this, powdermetallurgist has devoted much into minimized porosity because of higher porosity results inlower values in all mechanical properties of sintered steels.  In comparison with thenumerous studies concerned with other mechanical properties, the influence of porosity onwear behavior of sintered steels has not been extensively investigated.  The principalfactors that influence the sliding wear of the composites include: extrinsic factors such assliding distance, sliding velocity, applied load, atmosphere temperature, etc. and intrinsicfactors such as reinforcement type, shape, size, volume fraction and distribution, interfacebetween reinforcement and matrix, matrix material, heat treatment, porosity, etc.  The useof different copper and nickel particle sizes provided the ability to modify the porosity sizeand spacing.  Lee et al.  studied the effect of sintered porosity in powder metallurgy(PM) 6061 monolithic alloy and 6061: SiCp composites on dry abrasive wear, indicating thatthe wear rate of 6061 alloy increases drastically with increasing porosity, while for itscomposites, the porosity effect is not significant.The effect of porosity on the wear and friction of metals has been studied byVardavoulias et al. . They claimed that the pores enhance the surface roughness of thematerials and decrease the real area of contact between two sliding surfaces and consequentlyincrease the contact pressure and promote particle detachment during sliding. Suh  hasargued that the increase in porosity content of the composite reduces the required length ofcrack propagation to link-up with other cracks in order to cause delamination. Thus, porositydecreases the wear resistance and coefficient of friction of the composite. For differentsintered composites materials those effects are not constant depending on factors such as thecomposition and heat treating condition. Therefore, until now, it has been very difficult tomake a universal conclusion about the influence of pores on various sintered materials.In this paper, a careful evaluation of the samples wear behavior before and afterpractical application was done. The influence of sintering temperature on the porosity duringthe dry sliding wear behavior of sintered novel Cu-based composite train brake material wasinvestigated.2. EXPERIMENTAL DETAILS2.1 Sample preparationThe specimens used for this study are made by powder metallurgy technique, whichprocess includes mixing, compacting and sintering. The first step was the selection of powdermaterials categorized under based metal as the matrix, frictional components, lubricants andalloying elements. These were based on the outcome of Kryachek  review and Yao etal[8,9]. The newly developed bronze based brake pad powder material with its chemicalcomposition is given in Table 1.
3. International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 –6340(Print), ISSN 0976 – 6359(Online) Volume 4, Issue 2, March - April (2013) © IAEME523Table 1. Chemical compositions of material in mass (wt. %)Ingt: Matrix FrictionalcomponentLubricant component AlloyingelementCu (SiO2 & Fe) (Graphite &MoS2) (Mn & Sn)Wt%. 50-60 15-20 15-20 5.0The powders listed in Table 1 were weighed in a Sartorius BS224 S (Max 220gd=0.0001g) with their given proportion, the well prepared powder were mixed in a V-conemixer or double cone mixture machine. The rotating speed of double cone mixture wasmaintained at 150 rpm for nine hours. After the mixing process, the mixtures were compactedin a hardened steel die using a hydraulic press machine (SANS DCS-300 Digital HydraulicCompacting machine) under the pressure of 650Mpa.The compacts were subsequently transferred into a sintering furnace for sintering. Thesintering took 90 mins in a controlled atmosphere furnace saturated with carbon at 850-950oCat 0.01MPa constant pressure. The sintered materials were then driven out when oil-cooled.Finally, the resulting rectangular bar with thickness of 5mm was cut and grounded to a size of14mm × 14mm test specimens. Nine pairs of specimens were prepared for the friction andwear test.2.2 Testing ProceduresI. Characterisation testThe density of friction materials was determined according to a procedure proposed inASTM D792, which is based on Archimedes’ principle. This was done on all the samples atdifferent sintering temperatures and the average results are recorded in Table 3a.A digital microhardness tester HVS - 1000 instrument was used for the hardness and thehardness values were taken in the Vickers scale using 10N within 20 seconds. Prior to thehardness test, the samples were ground and polished with sand paper of grit 180, 240, 320,600, 800, 1000, and 1200 successively, and were also cleaned in alcohol in an ultrasoniccleaner. For each specimen, the hardness measurements were repeated ten times and anaverage of the ten was taken.A microstructure and tribosurfaces analysis was carried out with OM and SEM. Anoptical microscope (OM) and a scanning electron microscope (SEM) were employed toexamine microstructures of the specimen before and after the wear test. The surfaces of thespecimens were first polished with sand paper of grit 180, 240, 320, 600, 800, 1000, and 1200successively, followed by two polishing stages of 3µm and 0.05µm, respectively. The OMand the SEM helped analyze the nature of the microstructure for the likely pores availableand the wear surfaces, and they were done both before and after the wear test.II. PERFORMANCE TESTThe schematic diagram of the test rig is shown in Figure 1. During the tribotests, theperformance test includes the determination of coefficient of friction, friction force, wear lossand type of wear. These were tested according to the China National Standard GB5763-1998using an X-MSM Constant Speed Friction Material Tester with constant speed 7.54ms−1 andconstant pressure 3.13MPa. As a rotor, the disc made of cast iron (grade HTA5/HB withBrinell hardness in the range of 196) was used. The test rig is composed of the followingparts: the control and monitoring unit; the disc; and the sample holder. The friction test was
4. International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 –6340(Print), ISSN 0976 – 6359(Online) Volume 4, Issue 2, March - April (2013) © IAEME524performed at these selected temperatures (150, 200, 250, 300 and 350oC). Two specimenswere pressed against a gray cast iron rotating disk with a total contact area of approximately3.92cm2and rotated for 5000 revolution. The machine was originally made to apply 0.98MPaand cover 25×25mm of surface area. Modification of the sample holder was done, reducingthe surface area to 14×14 mm and thereby increasing the pressure on the sample to 3.13MPa.The friction coefficient data was obtained automatically by the tester. Five samplepairs were tested for each specimen and an average of the experimental data was taken as theresult. The wear coefficient k in mm3N−1m−1was calculated after 5000 revolutions of thedisc. Since the system cannot measure the wear loss directly, the volume wear rate by pad-on-disk wear testing (ASTM G99-95a) was used.Figure 1 Schematic Diagram of Test RigIt is now generally recognized that materials suitable for unlubricated tribologicalapplication (e.g. bearing, brake, wheel/rail, cam/tappet, piston/cylinder, work piece/tool, etc.)under the operating conditions (load Fa, speed v, temperature T, operating duration t, slidingdistance s), various friction and wear processes may occur and must fulfill the followingcriteria:..distslidingloadvolumewearcoeffwear×= (1)afforcefrictionaveragechangevolumeRnk,21×=π(2)the volume change is A(d1-d2).where R is the distance from the center of the rotating disk to the center of thespecimen (=0.15m), n is the number of rotations of the disk during testing (5,000 rev), A isthe area of the specimen (196mm2), d1 is the average thickness of the specimen before theexperiment (mm), d2 is the average thickness of specimen after the experiment (mm), and fais the automatically obtained average force of sliding friction (N) from the test rig. They wereobtained at temperatures of 100, 150, 200, 250, 300 and 350oC, respectively. The test rig wasequipped with a temperature control unit with a pump to circulate water under the disc tomaintain a controlled temperature. The average force was also recorded from the test rig atevery operating temperature. The volume change was obtained by calculating the difference
5. International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 –6340(Print), ISSN 0976 – 6359(Online) Volume 4, Issue 2, March - April (2013) © IAEME525between initial volume before test and the final volume after test. These and the otherparameters of the test rig were entered into equation (2) to obtain the results in Table 3.Also, wear numbers were also adopted. These were calculated, and used as a means ofknowing the wear resistance level of the design material. The mass of the specimen wasmeasured before and after the wear test to obtain the mass loss after 5,000 revolutions, attemperatures of 100, 150, 200, 250, 300 and 350oC, respectively. The densities were obtainedby the procedure proposed by ASTM D792 after the tribo test. This was done and the wearnumber was obtained as:VolumelossMassDensityWnumberWear n1)( == (3)where Wn is the wear number. Physically, it is per unit volume of the sample. Thehigher the wear number, the more effective the wear resistance of the material . Theresults are tabulated in Table 3.General porosity means the fraction of pore volume to the total volume. The porositycalculations were done using equation (4) after obtaining the various densities.1001, ×−=tPPorosityρρ(4)where, P is the porosity, ρ is the density of brake material and ρt is the density ofcorresponding bulk material.III. TEST CONDITIONAll tests were done under strict laboratory environmental and experimental standards.During the experiments, a constant rotation of 480rpm was maintained (sliding velocities of7.54ms-1); and the constant pressure was 3.13MPa based on the surface area of the specimen.The test rig is equipped with a temperature controlling unit with a pump to circulate waterunder the disc to maintain a controlled temperature.1. RESULTS AND DISCUSSION3.1. Porosity Effect on Friction and Worn surfaceThe effect of porosity and the sintering temperature on friction and worn surfaces ofthe sintered Cu-based composite rubbing against a rotor, the disk made of cast iron (gradeHTA5/HB with Brinell hardness in the range 196), are shown at figure 3. The worn surfacesof the composite specimen and wear debris were examined by SEM. The operating conditionfor pressure and sliding speed for all the samples are 3.13MPa and 7.4m/s.The typical SEM microphotographs of the worn surface for Cu-based composite are shown inFigure 3(a) to (c). The sections marked A on the microphotograph indicates the destructivewear sections during the tribo testing. The B sections are the relatively medium wearsurfaces, which indicate mild wear occurred during sliding. The section C has low wearsurface, glassy luster and integrated friction film, which shows this section has better wearresistance property. The surface sintered at 850oC (a) containing 17.53% porosity, showsabrasive scratches, indicating abrasive wear. The groove (in a) reveals plowing wear alsooccurred during sliding; this is material displacement to the side of the wear track. Thesurface sintered at 900oC (b) containing 15.82% porosity, shows flake-like fragments, and
6. International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 –6340(Print), ISSN 0976 – 6359(Online) Volume 4, Issue 2, March - April (2013) © IAEME526pits. These are a result of stress caused by high pressure exerted on the material duringoperation which results in delamination wear of medium-large flake-like fragments. Thelarger the flakes the more severe the delamination and therefore the greater the rate of wearobserved. The surface (c), sintered at 950 oC containing 14.04% porosity, shows ironparticles rich in carbon on the surface. The iron rich carbon formation increased resistance towear and this resulted in a very smooth surface as shown.The higher the porosity value of the samples, the lower coefficient of friction, lowerwear number and high wear coefficient resulting to high volume loss.From the discussions above, the general observation of the worn surfaces may be groupedinto three types; namely, destructive wear (found mostly on (a) and (b)); medium wear(mostly on (a) and (c)); and low wear (only on (c)).Fig. 3 Shows cross-sectional SEM micrograph of the nature of smoothness of frictionsurfaces at different sintering temperatures: (a) 850oC, (b) 900oC and (c) 950oC.3.2. Porosity Effect on Hardness and WearTable 2 shows the physical properties of the Cu-based composite. The wear ratechanges through the repeated contact process under constant load and velocity (3.13PMa and7.54m/s respectively) . Wear rates are often quoted in terms of a wear coefficient ordimensionless wear coefficient as derived from the Archard treatment of wear processes .The average hardness values measured with a Vickers hardness tester (Table 3) on all thematerials shows a similar tendency as the results of the sintering as shown in Figure 3. Thematerials with less porosity and sintered at high sintering temperature exhibited high hardnessas shown in Table 3 with low porosity at low sintering temperature. This confirmed the factthat, porosity influences the hardness, and therefore, affects the rate of wear of the material.From the same table, the wear rate was also greatly affected by the porosity values obtainedat their respective sintering temperatures.The wear volume rate (Vw) is calculated as shown in equation (1); where K is the wearcoefficient (dimensionless), W the normal load and H the hardness. The Archard treatment ofwear has been shown to be valid for cases where mechanical influences are dominant .Wear is often associated with hardness of the materials in contact. Basically, the harder thematerial, the more wear resistant it is, but it is also more brittle and therefore more sensitiveto the detachment of particles. According to Table 3, the lowest wear rate was observed at the950oC sintered material. This could be attributed to the fact that there was sufficient heatingto reduce porosity, which also brought about increase in hardness to optimize the wearproperties of the material.
7. International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 –6340(Print), ISSN 0976 – 6359(Online) Volume 4, Issue 2, March - April (2013) © IAEME527Table 2 Physical properties of Cu-based compositeRule Of Mixture( )3. −cmgtρ 3.973.7 −cmgExperiment DataAverage ( )3. −cmgρ 6.714 3. −cmgAverage Microhardness (HV) 294Average Porosity %, −=tPρρ1 15.79%Table 3. Properties of the Cu-based composite materialSint.Tem.TsinDensity, ρ Porosity, P Hardness,HvWear Coeff.kWear num.WnCoeff.Frict. µ850oC 6.51 17.53 272 0.000154 8.7191 0.336900oC 6.71 15.82 287 0.000166 9.8499 0.343950oC 6.85 14.04 304 0.000044 10.128 0.4043.3. Abrasive Surfaces ClassificationIn view of the advancement of technology, the application of computer-basedtechnology and image-processing methods have lead to a fully automated classificationsystem of tribological surfaces. Such a system has been useful in classifying (i) surfacesduring manufacturing processes (quality control), (ii) wear surfaces in the failure analysis ofengineering components, or (iii) wear particles in machine condition monitoring. The hybridfractal-wavelet method is used here to demonstrate how an unknown abrasive surface can beclassified into one of three classes of abrasive surfaces . 3-D surface morphology imagesare shown in Figure 4 to identify the different kinds of abrasive surfaces.In Figure 4, our investigation shows that the abrasive surfaces can be classified intothree divisions, named as smooth abrasive surface (mirror surface and integrated frictionfilm) which has better wear resistance property because it demonstrated minimal wear rate,rough abrasive surface (rough surface) indicates moderate wear rate and a highly abrasivesurface (much rough surface) showing excessive wear. Examples of the 3-D surfacemorphology images of the surface from each division are shown in Figure 4.
8. International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 –6340(Print), ISSN 0976 – 6359(Online) Volume 4, Issue 2, March - April (2013) © IAEME528Figure 4 shows 3-D surface morphology images of the surface (a) at 850 oC, (b) at 900 oCand (c) at 950 oC.The (a) is observed to be the one with a highly abrasive surface; this is as a result ofhaving fewer peaks that are ironic or hard to withstand pressure from the braking system. The(b) was also observed as the rough abrasive surface with moderate peaks withstanding theexerted pressure of the braking system. The (c) is the one that was observed as having enoughironic peaks to withstand the exerted pressure and therefore given a smooth abrasive surface.4. CONCLUSIONThe wear resistance properties of the novel Cu-based composite material against acast iron disc (grade HTA5/HB with Brinell hardness in the range 196) tested under a fulllaboratory condition, reveals a strong influence of porosity over the mechanical andtribological characteristics of the material. Investigation and observations concerning theeffect of porosity on the mechanical and tribological characteristics have led to the followingconclusions:The porosity level affects the mechanical properties. High porosity is not the best ifoptimizing the performance of the novel material, which leads to weakening of the materialsas a result of low sintering temperatures but this can be further improved and considered formanufacturing commercial brake pads. On the other hand, low porosity samples gave a highresistance to wear. This was as a result of the high sintering temperature which ensuredcomplete diffusion.Much lower wear coefficient, high wear number and high coefficient of friction wereobtained at low porosity samples (14.04% at 950oC) tested. These show high resistance towear; given good tribological characteristics and good mechanical properties.The dominant wear mechanisms found were plowing, delamination and abrasivewear. Abrasive wear and the delamination wear were the main cause of high wear coefficient,low wear number and low coefficient of friction. The nature of abrasive surfaces observedwere classified into three divisions, namely, smooth abrasive surfaces (mirror surface andintegrated friction film) which has better wear resistance properties because it demonstratesminimal wear rate; the rough abrasive surface (rough surface) indicates moderate wear rate;and lastly, the highly abrasive surface (much rough surface) showing excessive wear and hasa high degree of surface destruction. This is as a result of the rate of wear that occurredduring the dry sliding.
9. International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 –6340(Print), ISSN 0976 – 6359(Online) Volume 4, Issue 2, March - April (2013) © IAEME5295. ACKNOWLEDGMENTWe are grateful to the staff of The Key Laboratory of Specially Functional Materialsand Advanced Manufacturing Technology, Ministry of Education, South China University ofTechnology. We are also value the support of the staff of the Analytical and Testing Centerof South China University of Technology particularly Prof. Zhang Da Xue and Mr. Zhu FanKang (Chang Zhang) where we carried out the Experiments and the test.6. REFERENCES J. Wang, Y. He, and H. Danninger, Influence of Porosity on the Sliding Wear Behaviorof Sintered Fe-1.5Mo-0.7C Steels, ASM International, JMEPEG (2003) 12:339-344 M. Gui, S. B. Kang, J. M. Lee, Influence of porosity on dry sliding wear behavior inspray deposited Al–6Cu–Mn:SiCp composite, Materials Science and Engineering,A293 (2000) 146–156 T. M. Cimino, A. H. Graham and T. F. Murphy, The effect of microstructure and poremorphology on mechanical and dynamic properties of ferrous P/M materials, Presentedat pM2TEC 98 H.L. Lee, W.H. Lu, S.L. Chan, Abrasive wear of powder metallurgy Al alloy 6061-SiCparticle composites. Wear 159 (1992) 223 M. Vardavoulias, C. Jouannt-Tresy, M. Jeandin, Sliding wear behaviour of ceramicparticle reinforced high-speed steel obtained by powder metallurgy, Wear 165 (1993)141–149. N.P. Suh, An Overview of the Delamination Theory of Wear, Wear 44 (1977) 1–16. V. M. Kryachek, Sintered Metals and Alloys Friction Composites: Traditions and NewSolutions (Review). Powder Materials, Powder Metallurgy and Metal Ceramics, Vol.43, Nos. 11-12, 2004 Spring Science + Business Media, Inc. Xiong X., Sheng H, Chen J, Yao P, Effects Of Sintering Pressure And Temperature onMicrostructure and Tribological Characteristic of Cu-Based Aircraft Brake Material,Trans. Nonferrous Met. Soc. China 17(2007) 669-675 Yao P, Sheng H, Xiong X., Huang B., Worn Surface Characteristics of Cu-BasedPowder Metallurgy Brake for Aircraft, Trans. Nonferrous Met. Soc. China 17(2007) 99-103. Kato K,. Classification of Wear Mechanisms/Models, Wear – Materials, Mechanismsand Practice, Edited by G. Stachowiak , 2005, 9-20,. Williams J. A., Engineering Tribology Oxford Science Publications, Oxford UniversityPress, New York 1994. Neville A. and Morina A., Wear and Chemistry of Lubricants, Wear – Materials,Mechanisms and Practice, Edited by G. Stachowiak , 2005, 71-94. G. W. Stachowaik, G. B. Stachowiak, D. De Pellegrin, P. Posiadlo. Characterizationand Classification of Abrasive Particles and Surfaces, Wear–materials, mechanisms andpractice. Edited by G. Stachowiak 2005 339-368. ASTM B611. P. Kurmi, S. Rathod and P. Jain, “Abrasive Wear Behavior of 2014al-Tic in SituComposite”, International Journal of Mechanical Engineering & Technology (IJMET),Volume 3, Issue 3, 2012, pp. 229 - 240, ISSN Print: 0976 – 6340, ISSN Online:0976 – 6359.